Seoul National University System Health & Risk Management

## Chapter 9. Fatigue of Materials:

Introduction and Stress-Based Approach

Seoul National University System Health & Risk Management

CHAPTER 9 Objectives

• Explore the cyclic fatigue behavior of materials as a process of progressive damage leading to cracking and failure

• Fatigue trends for variables such as stress level, geometry, surface condition, environment, and microstructure

## • Review laboratory testing in fatigue, and analyze typical test data to obtain stress-life curves and evaluate mean stress effects.

• Apply engineering methods to estimate fatigue life, including the effects of mean stress, multiaxial stress, and variable-level cyclic loading

• Evaluate safety factors in stress and in life.

Contents

1 Introduction

2 Definitions and Concepts

3 Sources of Cyclic Loading

## 4 Fatigue Testing

5 The Physical Nature of Fatigue Damage

6 Trends in S-N Curves

7 Mean Stresses

8 Multiaxial Stresses

9 Variable Amplitude Loading

Contents

1 Introduction

2 Definitions and Concepts

3 Sources of Cyclic Loading

4 Fatigue Testing

5 The Physical Nature of Fatigue Damage

6 Trends in S-N Curves

## 7 Mean Stresses

8 Multiaxial Stresses

9 Variable Amplitude Loading

Fatigue Failure: de Havilland Comet disaster

• Three de Havilland Comet passenger jets broke up in mid-flight and **crashed within a few months in **
**1954.**

• The failure was a result of **metal fatigue in the airframes caused by the repeated pressurisation and de-**
**pressurisation **of the aircraft cabin.

• Unlike drill riveting, the imperfect nature of **the hole created by punch riveting **caused manufacturing
defect cracks which may have caused the start of fatigue cracks around the rivet.

• The stresses around pressure cabin apertures were considerably higher than anticipated, especially around sharp-cornered cut-outs, such as windows.

• Systematic tests were conducted on a fuselage immersed and pressurised in a water tank.

*http://en.wikipedia.org/wiki/Fatigue_(material)

## 9.1 Introduction – What is Fatigue?

• Purely static loading is rarely observed in modern engineering

components or structures. The majority of structures involve parts subjected to fluctuating or cyclic loads .

• Such loading induces fluctuating or cyclic stresses that often lead to microscopic damage to the materials.

• Accumulated microscopic damage develops into a crack or other macroscopic damage that leads to failure of the structure by fatigue .

### Figure 9.2 Figure 9.16

≈ 414Mpa

## 9.1 Introduction – What is Fatigue?

• From 80% to 95% of all structural failures occur through a fatigue mechanism.

• For centuries, it has been known that a piece wood or metal can be made to

break by repeatedly bending it back and forth with a large amplitude . However, it came as something of a surprise when it was discovered that repeated loading produced fracture even when the stress amplitude was apparently well below the elastic limit of the material (or ultimate strength ).

**Figure. **Representation of uniaxial stress-strain

relationship for 7075-T6 aluminum alloy* **Figure 9.4**

## < The Stress-Strain Curve and S-N Curve for 7075-T6 Al>

The stress below elastic

limit or ultimate strength

9.1 Introduction – History of Fatigue

• In 1837, Wilhelm Albert published the first article on fatigue, establishing a correlation between applied loads and durability.

• In 1839, Jean-Victor Poncelet, designer of cast iron axles for mill wheels, officially used the term " fatigue " for the first time in a book on mechanics.

## • In the 1850s, August Wöhler initiated the development of design strategies for fatigue and identified the importance of cyclic and mean stresses.

**Figure. **Albert's fatigue tests of mining chains, sketch

*http://www.atzonline.com/index.php;do=show/site=a4e/sid=GWV/alloc=38/id=61/special=Special+Simulation

9.4 Fatigue Testing

**Figure 9.11 **Rotating cantilever beam fatigue

testing machine used by **Wöhler. ** **Figure 9.12 **The **R. R. Moore **rotating beam
fatigue testing machine

## < Principle of fatigue testing machine>

9.1 Introduction -

3 major approaches analyzing fatigue failure

• Stress-based approach (Chapters 9-11)

– Analysis based on the nominal (average) stresses in the affected region of the engineering component.

– The nominal stress that can be resisted under cyclic loading is determined by considering mean stresses and by adjusting for the effects of stress raisers, such as grooves, holes, fillets, and keyways.

## • Strain-based approach (Chapter 14)

– More detailed analysis of the localized yielding that may occur at stress raisers during cyclic loading

• Fracture mechanics approach (Chapter 11)

– Specifically treats growing cracks by the methods of fracture mechanics

Stress-based approach

• The stress-life, or S-N method was the first approach used in an attempt to understand and quantify metal fatigue.

## • The basis of the stress-life method is the Wöhler or S-N diagram, which is a plot of alternating stress, S, versus cycles to failure, N.

• The most common procedure to obtain S-N data is the rotating bending test (R. R. Moore test).

• If S-N test data are found to approximate a straight line on a log-linear plot (or log-log), those can be fitted to obtain a mathematical

representation of the curve.

Stress-based approach

• One of the major drawbacks of the stress-life approach is that it ignores true stress-strain behavior and treats all strains as elastic.

## • The simplifying assumptions of the S-N approach are valid only if the plastic strains are small.

• At long lives most steels have only a small component of cyclic strain which is plastic (in some cases it is effectively too small to measure) and the S-N approach is valid.

• The stress-life method does not work well in low-cycle applications,

where the applied strains have a significant plastic component. In this

range a strain-based approach is more appropriate.

## Contents

1 Introduction

2 Definitions and Concepts

3 Sources of Cyclic Loading

4 Fatigue Testing

5 The Physical Nature of Fatigue Damage

6 Trends in S-N Curves

7 Mean Stresses

8 Multiaxial Stresses

9 Variable Amplitude Loading Variable Amplitude Loading

10

9.2.1 Description of Cyclic Loading

**Figure 9.2 **Constant amplitude cycling and the associated nomenclature. Case (a) is completely
reversed stressing, σ_{m}= 0; (b) has a nonzero mean stress σ_{m}; and (c) is zero-to-tension stressing,
σmin= 0.

## Tension – Compression Loading

Tension – Tension Loading

9.2.1 Description of Cyclic Loading

< Completely Reversed Cycling>

σ

_{𝑚𝑚}

= 0 𝑜𝑜𝑜𝑜 𝑅𝑅 = −1

< Zero-to-Tension Cycling>

σ

_{𝑚𝑚𝑖𝑖𝑖𝑖}

= 0 𝑜𝑜𝑜𝑜 𝑅𝑅 = 0 σ

_{𝑎𝑎}

= Δσ

2 =

σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

− σ

_{𝑚𝑚𝑖𝑖𝑖𝑖}

2 σ

_{𝑚𝑚}

= σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

+ σ

_{𝑚𝑚𝑖𝑖𝑖𝑖}

2 σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

= σ

_{𝑚𝑚}

+ σ

_{𝑎𝑎}

σ

_{𝑚𝑚𝑖𝑖𝑖𝑖}

= σ

_{𝑚𝑚}

− σ

_{𝑎𝑎}

Stress Ratio, 𝑅𝑅 =

_{σ}

^{σ}

^{𝑚𝑚𝑚𝑚𝑚𝑚}

𝑚𝑚𝑚𝑚𝑚𝑚

Amplitude Ratio, 𝐴𝐴 =

_{σ}

^{σ}

^{𝑚𝑚}

𝑚𝑚

σ

_{𝑎𝑎}

= Δσ 2 =

σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

2 (1 − 𝑅𝑅) σ

_{𝑚𝑚}

= σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

2 (1 + 𝑅𝑅) 𝑅𝑅 = 1 − 𝐴𝐴

1 + 𝐴𝐴 𝐴𝐴 = 1 − 𝑅𝑅 1 + 𝑅𝑅 (9.1)

(9.2)

(9.3) (9.4)

-> Describing Cyclic Loading

9.2.2 Point Stresses vs. Nominal Stresses

**Figure 9.3 **Actual and nominal stresses
for (a) simple tension, (b) bending, and (c)
a notched member.

Stress at a point, σ Nominal or Average stress, S

- Actual stress occurred at a point - Calculated stress from force or moment or their combination as a matter of convenience and is only equal to σin certain situations

-> Simple Axial Loading -> Complicated Bending, notched member (except where it is truly appropriate to use σ)

Actual Stress distribution (σ) Hypothetical Distribution

(associated with nominal stresses S) Elastic Stress Concentration

<Elastic Behavior> <Plastic Behavior>

## 9.2.3 Stress Versus Life (S-N) Curves

**Figure 9.4** Stress versus life (S-N) curves from rotating bending tests of unnotched specimens
of an aluminum alloy. Identical linear stress scales are used, but the cycle numbers are plotted
on a linear scale in (a), and on a logarithmic one in (b). (Data from [MacGregor 52].)

• The results of tests from a number of different stress levels may be plotted to obtain a stress-life curve, also called an S-N curve.

• If the test is repeated at a higher stress level, the number of cycles to failure will be smaller.

linear scale Logarithmic scale

Zero mean stress No stress raiser

## 9.2.3 Stress Versus Life (S-N) Curves

• B, Fatigue Strength

– A stress amplitude value from an S-N curve at a particular life of interest.

• A, Endurance Limit, S

_{e}

(or σ

_{erb}

, Fatigue Limit) for most steels

– If the applied stress level is below the endurance limit of the material, the structure is said to have an safe and infinite life.

## – The endurance limit is due to interstitial elements, such as carbon or

nitrogen in iron, which pin dislocations. This prevents the slip mechanism

that leads to the formation of micro cracks.

9.6.1 Trends with Ultimate Strength

**Figure 9.24 **Rotating bending
fatigue limits, or failure stresses for
10^{7}to 10^{8}cycles, from polished
specimens of various ferrous metals.

The slopes *m*_{e}= *σ*_{erb}/*σ*_{u} indicate the
average and approximate extremes
of the data for *σ*_{u} < 1400 MPa.

## < Endurance Limit Related to Ultimate Strength>

𝑆𝑆

_{𝑒𝑒}

≈ 0.5 × 𝑆𝑆

_{𝑢𝑢}

𝑓𝑓𝑜𝑜𝑜𝑜 𝑆𝑆

_{𝑢𝑢}

≤ 200𝑘𝑘𝑘𝑘𝑘𝑘 𝑆𝑆

_{𝑒𝑒}

≈ 100𝑘𝑘𝑘𝑘𝑘𝑘 𝑓𝑓𝑜𝑜𝑜𝑜 𝑆𝑆

_{𝑢𝑢}

> 200𝑘𝑘𝑘𝑘𝑘𝑘

= 1379Mpa

-> A reasonable degree of ductility is helpful in providing resistance to cyclic loading.

-> Too high-strength materials can lead to fatigue failures.

Most steels have limited ductility at high-strength levels

### Fatigue Ratio of 0.5

## 9.2.3 Stress Versus Life (S-N) Curves

**Figure 9.5 **Rotating bending S-N curve for unnotched specimens of a steel with a distinct fatigue
limit. (Adapted from [Brockenbrough 81]; used with permission.)

Fatigue limits

9.2.3 Stress Versus Life (S-N) Curves

(9.5) Log-linear plot, σ

_{𝑎𝑎}

= 𝐶𝐶 + 𝐷𝐷𝐷𝐷𝑜𝑜𝐷𝐷𝑁𝑁

_{𝑓𝑓}

Log-log plot, σ

_{𝑎𝑎}

= 𝐴𝐴𝑁𝑁

_{𝑓𝑓}

^{𝐵𝐵}

(9.6)

(9.7) Different Log-log plot, σ

_{𝑎𝑎}

= σ

_{𝑓𝑓}

^{′}

(2𝑁𝑁

_{𝑓𝑓}

)

^{𝑏𝑏}

(9.8) 𝐴𝐴 = 2

^{𝑏𝑏}

σ

_{𝑓𝑓}

^{′}

𝐵𝐵 = 𝑏𝑏

### Figure 9.5

**Table 9.1 **Constants for stress-life curves for
various ductile engineering metals, From
tests at zero mean stress on unnotched axial
specimens

## 9.2.4 Safety Factors for S-N Curves

**Figure 9.6 **Stress–life curve and the stress
amplitude and number of cycles expected in
actual service, σ_{a}and N, giving safety factors X_{s} in
stress and X_{N}in life.

(9.9) The safety factor in stress, 𝑋𝑋

_{𝑆𝑆}

=

^{σ}

_{�σ}

^{𝑚𝑚1}

𝑚𝑚

, (𝑁𝑁

_{𝑓𝑓}

= 𝑁𝑁) �

(9.10) The safety factor in life, 𝑋𝑋

_{𝑁𝑁}

=

^{𝑁𝑁}

_{𝑁𝑁}

_{�}

^{𝑓𝑓𝑓}

, (σ

_{𝑎𝑎}

= �σ

_{𝑎𝑎}

)

Contents

1 Introduction

2 Definitions and Concepts

3 Sources of Cyclic Loading

## 4 Fatigue Testing

5 The Physical Nature of Fatigue Damage

6 Trends in S-N Curves

7 Mean Stresses

8 Multiaxial Stresses

9 Variable Amplitude Loading Variable Amplitude Loading

10

9.3 Sources of Cyclic Loading

• Some practical applications involve cyclic loading at a constant amplitude, but irregular load versus time histories are more commonly encountered.

## • Working loads and vibratory loads are the cyclic loads causing fatigue failure. However, the damage due to static loads and accidental loads also plays an additional role.

Loads Characteristics

Static loads Do not vary and continuously present

Ex) Highway bridge, The always-present weight of the structure and roadway Working loads Change with time and incurred as a result of the function performed by the

component

Ex) The weight of vehicles

Vibratory loads Relatively high-frequency cyclic loads from environment or as a secondary effect of the function of the component

Ex) tires interacting with the roughness of the roadway, bouncing of vehicle, wind turbulance

Accidental loads Rare events occurring under abnormal circumstances Ex) Vehicle accident, Earthquake

## I-5 Skagit River Bridge collapse: Accidental loads

A collapsed section of the Interstate 5 bridge over the Skagit River ( north of Seattle) is seen in an aerial view Friday, May 24, 2013.

*http://www.columbian.com/news/2013/may/24/north-wash-i-5-bridge-collapse-caused-oversize-loa/

9.3 Sources of Cyclic Loading

**Figure 9.7 **Sample record of stresses at the steering knuckle arm of a motor vehicle, including
the original stress–time history (a), and the separation of this into the vibratory load due to
roadway roughness (b) and the working load due to maneuvering the vehicle (c). (From
[Buxbaum73]; used with permission; first published by AGARD/NATO.)

Chassis Suspension

## Steering Knuckle arm

Contents

1 Introduction

2 Definitions and Concepts

3 Sources of Cyclic Loading

4 Fatigue Testing

5 The Physical Nature of Fatigue Damage

6 Trends in S-N Curves

7 Mean Stresses

8 Multiaxial Stresses

9 Variable Amplitude Loading Variable Amplitude Loading

10

Microscopic

Macroscopic

9.5 The (Microscopic) physical Nature of Fatigue Damage

## • When viewed at a sufficiently small size scale, all materials are

anisotropic and inhomogeneous. ( ∵ grain, crystal plane, voids, particles)

• As a result of nonuniform microstructure, stresses are distributed in a nonuniform manner when viewed at the micro size.

• Regions where the stresses are severe are usually the points where fatigue damage starts.

**Figure 9.16 **Photographs of broken 7075-T6 aluminum fatigue test specimens:

unnotched axial specimen, 7.6 mm diameter (left); and plate 19 mm wide with a round hole (right). In the unnotched specimen, the crack started in the flat region with slightly lighter color, and cracks in the notched specimen started on each side of the hole.

## 9.5 The (Microscopic) physical Nature of Fatigue Damage

• For ductile engineering metals, crystal grains that have an unfavorable orientation relative to the applied stress first develop slip bands.

• Additional slip bands form as more cycles are applied until saturation level.

• Individual slip bands become more severe, and some develop into cracks within grains, which then spread into other grains, joining with other similar cracks, and producing a large crack that propagates to failure.

**Figure 9.17 **The process of slip band damage during cyclic loading developing into a crack in an
Axial direction

## 9.5 The (Microscopic) physical Nature of Fatigue Damage

• For materials of somewhat limited ductility, such as high-strength metals, the microstructural damage is less widespread and tends to be

concentrated at defects in the materials.

• A small crack develops at a void, inclusion, slip band, grain boundary, or surface scratch, or there may be a sharp flaw initially present that is essentially a crack. This crack grows in a plane generally normal to the tensile stress until it causes failure.

Crack Started from the inclusion

**Figure 9.18 **Fatigue crack origin in an **Figure 1.8 **Development of a fatigue
crack during rotating bending of a

## 9.5 The (Microscopic) physical Nature of Fatigue Damage

**Figure 9.19 **Stress–life curves for completely reversed bending of smooth specimens, showing
various stages of fatigue damage in an annealed 99% aluminum (1230-0), and in a hardened
6061-T6 aluminum alloy.

< Material of Ductility> < Material of Limited Ductility>

9.5 The (Macroscopic) physical Nature of Fatigue Damage

**Figure 9.21 **Fracture surfaces for fatigue
and final brittle fracture in an 18 Mn steel
member.

## Tensile Direction

<Beach marks (the process of crack)>

(1) Growth rate change due to altered stress level, temperature, chemical environment

(2) Discoloration due to corrosion

<Slow and Smooth>

<Fast and Rough>

<Shear lip>

- Ductile material forms a shear lip,

inclined at approximately 45 degrees

## to the applied stress

9.5 The (Microscopic) physical Nature of Fatigue Damage

**Figure 9.21 **Fracture surfaces for fatigue
and final brittle fracture in an 18 Mn steel
member.

**Figure 9.22 **Fatigue striations spaced
approximately 0.12 μm apart, from a
fracture surface of a Ni-Cr-Mo-V steel.

<Striations>

- Ductile material often reveals

marks left by the progress of

## the crack on each cycle.

Contents

1 Introduction

2 Definitions and Concepts

3 Sources of Cyclic Loading

4 Fatigue Testing

5 The Physical Nature of Fatigue Damage

6 Trends in S-N Curves

7 Mean Stresses

8 Multiaxial Stresses

9 Variable Amplitude Loading Variable Amplitude Loading

10

9.6 TRENDS IN S-N CURVES

• S-N curves vary widely for different classes of materials.

## • The higher the S-N curve -> the more resistant to fatigue

**Figure 9.23 **Stress–life curves from cantilever bending of mineral and glass-filled thermosets
(solid lines) and unfilled thermoplastics (dashed lines).

No Endurance Limit

For Nonferrous metals

9.6 TRENDS IN S-N CURVES

Factors lowering the S-N curve Factors raising the S-N curve

- **Reduce the value of endurance limit**
- **Shorten the life**

- **Lowering the fatigue strength**

- **Increase the value of endurance limit**
- **Extension of the life**

- **Raising the fatigue strength**

## - High-strength material (limited-ductility material) - Tensile mean stress

- Stress raisers (notches, high stress concentration factor k

_{t}

)

- Harsh environment (high

temperature, salt solution, moisture and gases in air)

- Micro defects (larger size of

inclusions and voids, larger size of grains (annealing))

- High ultimate strength - Compressive mean stress

## - Dense network of dislocations

- Processing without decreasing the ductility (cold rolling, shoot

peening, carburization)

= (Moore endurance limit)

*e* *L* *G* *S* *T* *R* *e*

*S* *C C C C C S*′

Chapter Later on

9.6.1 Trends with Mean Stresses

**Figure 9.26 **Axial loading S-N curves at various mean stresses for unnotched specimens of an
aluminum alloy. The curves connect average fatigue strengths for a number of lots of material.

Compressive mean stress

Tensile mean stress

## 9.6.1 Trends with Member Geometry

**Figure 9.27 **Effects of notches having k_{t} = 1.6 and 3.1 on rotating bending S-N curves of an
aluminum alloy. (Adapted from [MacGregor 52].)

9.6.2 Effects of Environment

**Figure 9.28 **Effect of a salt solution similar to seawater on the bending fatigue behavior of an
aluminum alloy. (Data from [Stubbington61].)

9.6.2 Effects of Environment

**Figure 9.29 **Temperature and frequency effects on axial S-N curves for the nickel-base alloy
Inconel. (Illustration from [Gohn 64] of data in [Carlson 59]; used with permission.)

* cpm: harsh condition cycles per minute

## 9.6.3 Effects of Microstructure

**Figure 9.30 **Influence of grain size and cold work on rotating bending S-N curves for 70Cu-30Zn
brass. (From [Sinclair 52]; used with permission.)

Little Effect

Grain size, Dislocation, and Fatigue

What is the relationship between dislocation and fatigue failure?

• The life of fatigue has two parts, initiation and propagation.

• A dislocation plays a major role in the fatigue crack initiation.

• After a large number of loading cycles, dislocations pile up and form structures called persistent slip bands.

• Persistent slip bands are areas that rise above (extrusion) or fall below (intrusion) the surface of the component due to movement of material along slip planes.

• This leaves tiny steps in the surface that serve as stress raisers where fatigue cracks can initiate.

*https://www.ndeed.org/EducationResources/CommunityCollege/Materials/Structure/fatigue.htm

## Grain size, Dislocation, and Fatigue

Why is it so difficult for the dislocation to travel through the boundary and what other problems would face it if it were to jump the gap?

• Inside the grain boundary, the atoms are jumbled. As a result additional energy is required to force the dislocation through the boundary.

Why does the small grain size make material more resistant to fatigue failure?

• A dislocation could move from one atomic plane to another with the defect like a wave traveling over the sea.

• However, a dislocation cannot carry on moving forever.

• A dislocation will run into a grain boundary, and stuck here.

• If the grain size is decreased, there will be an increase in area of the grain boundary compared to the

number dislocations in the grain.

## 9.6.4 Residual Stress and Other Surface Effects

: Peening

9.6.4 Residual Stress and Other Surface Effects

**Figure 9.31 **S-N curves for zero-to-maximum bending, and residual stresses, for variously shot
peened steel leaf springs. (From [Mattson 59]; courtesy of General Motors Research Laboratories.)

9.6.5 Fatigue Limit Behavior

### Figure 9.5 Figure 9.4

## 9.6.5 Fatigue Limit Behavior

• Fatigue occurs below the fatigue limit

• Failure that begins from surface defects and failure that begins from internal nonmetallic inclusions

• If the fatigue process can somehow start, then it can proceed below the fatigue limit.

– Corrosion may cause small pits.

– Surface damage allows fatigue cracks.

## 9.6.5 Fatigue Limit Behavior

**Figure 9.32 **Stress–life curve extending into the very long life range for a bearing steel with

hardness HV = 778, corresponding to σ_{u} ≈ 2350 MPa, containing 1% carbon and 1.45% chromium.

9.6.5 Fatigue Limit Behavior

**Figure 9.33 **Stress–life data for a low-strength steel tested under constant amplitude cycling with
zero mean stress. Periodic overstrain tests included severe cycles applied every 10^{5} cycles, but
with their ΣN/Nfnot exceeding a few percent. (Data from [Brose 74].)

## 9.6.6 Statistical Scatter

**Figure 9.34 **Scatter in rotating bending S-N
data for an unnotched aluminum alloy.

(Adapted from [Grover 66] p. 44.)

**Figure 9.35 **Distribution of fatigue
lives for 57 small specimens of 7075-
T6 aluminum tested at S_{a}= 207 MPa
(30 ksi) in rotating bending.

Contents

1 Introduction

2 Definitions and Concepts

3 Sources of Cyclic Loading

4 Fatigue Testing

## 5 The Physical Nature of Fatigue Damage

6 Trends in S-N Curves

7 Mean Stresses

8 Multiaxial Stresses

9 Variable Amplitude Loading Variable Amplitude Loading

10

9.7.1 Presentation of Mean Stress Data

• One procedure used for developing data on mean stress effects is to select

several values of mean stress, running tests at various stress amplitudes for each of theses.

## • An alternative presentation means, a constant-life diagram, shows that to

maintain the same life, increasing the mean stress in the tensile direction must be accompanied by a decrease in stress amplitude.

**Figure 9.26 **Axial loading S-N curves at **Figure 9.37 **Constant-life diagram taken

σ

_{a }

-> 0, σ

_{m}

-> σ

_{u}

9.7.2 Normalized Amplitude-Mean Diagrams

**Figure 9.37 **Constant-life diagram taken

from the S-N curves **Figure 9.39 **Normalized amplitude-

mean diagram

## • On a constant-life diagram, σ

_{ar}

(or S

_{e}

) is thus the intercept at σ

_{m}

=0 of the curve for any particular life.

• The graph can be normalized by plotting values of the ratio σ

_{a}

/σ

_{ar}

versus the

mean stress σ

_{m. }

(σ

_{m}

, σ

_{a}

/σ

_{ar}

)

9.7.2 Normalized Amplitude-Mean Diagrams 9.7.1 Additional Mean Stress Equations

**Figure 9.39 **Normalized amplitude-
mean diagram

## • Several empirical relationships have been developed.

• For most fatigue design situations (i.e., small mean stress in relation to alternating stress), there is little difference in the theories.

Goodman (England, 1899)

Gerber (Germany, 1874)

Morrow (USA, 1960s)

- Conservative line

- Incorrect for compressive stress

- Using true fracture strength

9.7.4 Life estimates with Mean Stress

σ

_{𝑎𝑎𝑎𝑎}

= σ

_{𝑓𝑓}

^{′}

(2𝑁𝑁

_{𝑓𝑓}

)

^{𝑏𝑏}

= 1758(2𝑁𝑁

_{𝑓𝑓}

)

^{−0.0977}

𝑀𝑀𝑀𝑀𝑀𝑀 (9.7)

Example 9.3) The AISI 4340 Steel is subjected to cyclic loading with a tensile mean stress of σ

_{m}

## =200MPa. what life is expected if the stress amplitude is σ

_{a}

=450MPa?

Solution)

From Table 9.1 (p. 406), σ

_{𝑓𝑓}

^{′}

=1758, b=-0.0977

σ

_{𝑎𝑎𝑎𝑎}

= σ

_{𝑎𝑎}

1 − σ σ

^{𝑚𝑚}

_{𝑓𝑓}

^{′}

= 450 1 − 200

1758

= 507.8𝑀𝑀𝑀𝑀𝑀𝑀 (Morrow)

𝑁𝑁

_{𝑓𝑓}

= 166,000 𝐶𝐶𝐶𝐶𝐶𝐶𝐷𝐷𝐶𝐶𝑘𝑘

Contents

1 Introduction

2 Definitions and Concepts

3 Sources of Cyclic Loading

4 Fatigue Testing

5 The Physical Nature of Fatigue Damage

6 Trends in S-N Curves

7 Mean Stresses

8 Multiaxial Stresses

9 Variable Amplitude Loading

9.8 MULTIAXIAL STRESSES (Optional)

**Figure 9.40 **Combined cyclic pressure and steady bending of a thin-walled tube with closed ends.

## • Commonly, cyclic loadings cause complex states of multiaxial stress.

Examples)

– Fig 9.40: Combination of cyclic pressure “P” and steady bending “M” causes biaxial
stresses “σ_{1}, σ_{2}”.

– There are different stress amplitudes and mean stresses in two directions

Fluctuating Pressure

Steady Bending

9.8.1 One Approach to Multiaxial Fatigue (Optional)

• Assumption & Situation #1

– All cyclic loads are completely reversed and have the same frequency.

– No steady (noncyclic) load presents.

## • Effective stress amplitude, �𝝈𝝈

_{𝒂𝒂}

– The amplitudes of the principal stresses can be used to compute an *effective stress *
*amplitude*.

– Similar relationship employed for the octahedral shear yield criterion (Chapter 7, Eq 7.35)

– By using effective stress amplitude, the fatigue life ban be estimated for completely
reversed uniaxial stress. (σ_{m}=0)

σ

_{𝑎𝑎𝑎𝑎}

= σ

_{𝑎𝑎}

1 − σ

_{𝑚𝑚}

σ

_{𝑓𝑓}

^{′}

σ

_{𝑎𝑎𝑎𝑎}

= σ

_{𝑓𝑓}

^{′}

(2𝑁𝑁

_{𝑓𝑓}

)

^{𝑏𝑏}

(Morrow)

## 9.8.1 One Approach to Multiaxial Fatigue (Optional)

• Assumption & Situation #2

– If steady (noncyclic) loads are present

• Effective stress amplitude, �𝝈𝝈

_{𝒂𝒂}

– The amplitudes of the principal stresses can be used to compute an *effective stress *
*amplitude*.

• Effective mean stress, �𝝈𝝈

_{𝒎𝒎}

– Effective mean stress can be calculated from the mean stresses in the three principal directions

– By using effective stress amplitude & effective mean stress, the fatigue life ban be estimated.

σ

_{𝑎𝑎𝑎𝑎}

= σ

_{𝑎𝑎}

1 − σ

_{𝑚𝑚}

σ

_{𝑓𝑓}

^{′}

σ

_{𝑎𝑎𝑎𝑎}

= σ

_{𝑓𝑓}

^{′}

(2𝑁𝑁

_{𝑓𝑓}

)

^{𝑏𝑏}

(Morrow)

## Contents

1 Introduction

2 Definitions and Concepts

3 Sources of Cyclic Loading

4 Fatigue Testing

5 The Physical Nature of Fatigue Damage

6 Trends in S-N Curves

7 Mean Stresses

8 Multiaxial Stresses

9 Variable Amplitude Loading

9.9.1 The Palmgren-Miner Rule

• In practical applications, the variable amplitude of fatigue loadings exist.

## • The Palmgren(in 1920s)-Miner(in 1945) Rule

- 𝑁𝑁_{1}: the number of cycles by stress amplitude 𝜎𝜎_{𝑎𝑎1}

- 𝑁𝑁_{𝑓𝑓1}: the number of cycles to failure from the S-N curve for 𝜎𝜎_{𝑎𝑎1}
- 𝑁𝑁_{1}/𝑁𝑁_{𝑓𝑓1}: the fraction of the life

- Fatigue Failure is expected when such life fractions sum to unity.

- It is convenient to sum cycle ratios over one repetition for the summation to reach
unity. 𝐵𝐵_{𝑓𝑓}: the number of repetitions to failure

𝑁𝑁_{1}

𝑁𝑁_{𝑓𝑓1} + 𝑁𝑁_{2}

𝑁𝑁_{𝑓𝑓2} + 𝑁𝑁_{3}

𝑁𝑁_{𝑓𝑓3} +⋯ = � 𝑁𝑁_{𝑗𝑗}

𝑁𝑁_{𝑓𝑓𝑗𝑗} = 1, 𝑛𝑛

𝑁𝑁 = 𝐶𝐶𝐶𝐶𝐶𝐶𝐷𝐷𝐶𝐶 𝑜𝑜𝑀𝑀𝑟𝑟𝑘𝑘𝑜𝑜 ^{𝐵𝐵}𝑓𝑓 � 𝑁𝑁_{𝑗𝑗}
𝑁𝑁_{𝑓𝑓𝑗𝑗}

𝑜𝑜𝑖𝑖𝑒𝑒 𝑎𝑎𝑒𝑒𝑟𝑟.

= 1

**Figure 9.43 **Use of the Palmgren–Miner rule for life prediction for variable amplitude.

## 9.9.1 The Palmgren-Miner Rule

Example 9.8)

A Uniaxial stress repeatedly applied to an unnotched member made of the AISI 4340 Steel. Estimate the number of repetitions, 𝐵𝐵

_{𝑓𝑓}

, required to cause fatigue failure.

Solution)

From Table 9.1 (p. 406), σ

_{𝑓𝑓}

^{′}

=1758, b=-0.0977

σ

_{𝑎𝑎}

= (σ

_{𝑓𝑓}

^{′}

−σ

_{𝑚𝑚}

)(2𝑁𝑁

_{𝑓𝑓}

)

^{𝑏𝑏}

(9.23) (Morrow for nonzero mean stress) σ

_{𝑎𝑎}

= Δσ

2 =

σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

− σ

_{𝑚𝑚𝑖𝑖𝑖𝑖}

2

σ

_{𝑚𝑚}

= σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

+ σ

_{𝑚𝑚𝑖𝑖𝑖𝑖}

2

𝐵𝐵_{𝑓𝑓} = 1

∑ 𝑁𝑁_{𝑗𝑗}

𝑁𝑁𝑓𝑓𝑗𝑗 𝑜𝑜𝑖𝑖𝑒𝑒 𝑎𝑎𝑒𝑒𝑟𝑟.

= 1

1.388 × 10^{−5} = 72000𝑜𝑜𝐶𝐶𝑟𝑟.

9.9.2 Cycle Counting for Irregular Histories

• To predict the life of a component subjected to a variable load history, it is

## necessary to reduce the complex history into a number of events which can be compared to the available constant amplitude test data. This process of reducing a complex load history into a number of constant amplitude events involves what is termed cycle counting.

Figure 9.7 Figure 9.8

9.9.2 Cycle Counting for Irregular Histories

- Simplified Rainflow Counting for Repeating Histories

• In performing rainflow cycle counting, a cycle is identified or counted if it meets the criterion.

• A peak-vally-peak or vally-peak-valley combination is considered to contain a cycle

Figure 9.45 Definitions for irregular loading.

## Figure 9.46 Condition for counting a cycle with the rainflow method.

9.9.2 Cycle Counting for Irregular Histories

- Simplified Rainflow Counting for Repeating Histories

Figure 9.47 Example of rainflow cycle counting.

< Rainflow cycle counting>

(1) Assume that the stress history given is to be repeatedly applied.

(2) (a) -> (b) Arrange the history to start with either the maximum peak or the minimum valley.

(3) If Δσ_{YZ}≥Δσ_{XY}, then a cycle is

counted. And its peak and valley are assumed not to exist for further cycle counting .

(4) If Δσ_{YZ }<Δσ_{XY}, then no cycle can be
counted. And move ahead until a
count can be made

Combination Cycle Counts Range Mean

DE>EF 0

**EF**<FG 1 4.0 1.0

GH>HA 0

HA>AB 0

**AB**<BC 1 3.0 -0.5

Combination Cycle Counts Range Mean DG>GH

GH>HC 0

**HC<**CD 1 7.0 0.5

DG=**DG** 1 9.0 0.5

## 9.9.2 Cycle Counting for Irregular Histories

- Simplified Rainflow Counting for Repeating Histories

Figure 9.48 An irregular load vs.

time history from a ground

vehicle transmission, and a matrix giving numbers of rainflow cycles at various combinations of range and mean. The range and mean values are percentages of the peak load; in constructing the

## matrix, these were rounded to the discrete values shown. (Load

history from [Wetzel 77] pp. 15–

18.)

Thank You

Back Up

9.1 Introduction - Wind Turbines Fatigue

**Figure 9.1 **Large horizontal-axis wind turbine in
operation on the Hawaiian island of Oahu. The
blade has a tip-to-tip span of 98 m. (Photo courtesy
of the NASA Lewis Research Center, Cleveland, OH.)

## • Wind turbines are subjected to cyclic loads due to rotation and wind

turbulence, making fatigue a critical

aspect of the design of the blade and

other moving parts.

수식

σ

_{𝑎𝑎}

= Δσ 2 =

σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

− σ

_{𝑚𝑚𝑖𝑖𝑖𝑖}

2 σ

_{𝑚𝑚}

= σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

+ σ

_{𝑚𝑚𝑖𝑖𝑖𝑖}

2 σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

= σ

_{𝑚𝑚}

+ σ

_{𝑎𝑎}

σ

_{𝑚𝑚𝑖𝑖𝑖𝑖}

= σ

_{𝑚𝑚}

− σ

_{𝑎𝑎}

Stress Ratio, 𝑅𝑅 =

_{σ}

^{σ}

^{𝑚𝑚𝑚𝑚𝑚𝑚}

𝑚𝑚𝑚𝑚𝑚𝑚

Amplitude Ratio, 𝐴𝐴 =

_{σ}

^{σ}

^{𝑚𝑚}

𝑚𝑚

σ

_{𝑎𝑎}

= Δσ 2 =

σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

2 (1 − 𝑅𝑅) σ

_{𝑚𝑚}

= σ

_{𝑚𝑚𝑎𝑎𝑚𝑚}

2 (1 + 𝑅𝑅) 𝑅𝑅 = 1 − 𝐴𝐴

1 + 𝐴𝐴 𝐴𝐴 = 1 − 𝑅𝑅 1 + 𝑅𝑅 (9.1)

(9.2)

(9.3) (9.4)

(9.5) Log-linear plot, σ

_{𝑎𝑎}

= 𝐶𝐶 + 𝐷𝐷𝐷𝐷𝑜𝑜𝐷𝐷𝑁𝑁

_{𝑓𝑓}

Log-log plot, σ

_{𝑎𝑎}

= 𝐴𝐴𝑁𝑁

_{𝑓𝑓}

^{𝐵𝐵}

(9.6)

(9.7) Different Log-log plot, σ

_{𝑎𝑎}

= σ

_{𝑓𝑓}

^{′}

(2𝑁𝑁

_{𝑓𝑓}

)

^{𝑏𝑏}

(9.8) 𝐴𝐴 = 2

^{𝑏𝑏}

σ

_{𝑓𝑓}

^{′}

𝐵𝐵 = 𝑏𝑏 (9.9) The safety factor in stress, 𝑋𝑋

_{𝑆𝑆}

=

^{σ}

_{�σ}

^{𝑚𝑚1}

𝑚𝑚

, (𝑁𝑁

_{𝑓𝑓}

= 𝑁𝑁) �

(9.10) The safety factor in life, 𝑋𝑋

_{𝑁𝑁}

=

^{𝑁𝑁}

_{𝑁𝑁}

_{�}

^{𝑓𝑓𝑓}

, (σ

_{𝑎𝑎}

= �σ

_{𝑎𝑎}

)

## 열간압연 vs. 냉간압연

열간압연 강판 특성 냉간압연 강판

### 재결정온도 이상에서 압연 온도 재결정온도 이하에서 압연

성형이 쉬움 성형성 성형이 어려움

낮은 극한 응력 기계적 성질 높은 극한응력 흑피 형성(불순물 층)

-> 피로, 충격에 약함

불순물 표면 깨끗함

### (굳은 불순물 제거됨, 더 이상 불순물이 분리되지 않는 온도) 정수치 불가 가공 두께 두께 균일(분자 구조 안정)

-> 코일 형태 보관 가능

(Hot Rolled Steel Sheet)

(Cold Rolled Steel Sheet)

• Stress was used as the control parameter and stress-life (or S-N) curves characterized the material or component response to cyclic loading. This approach was used widely until the 1970s when the new methods started to be used by industry. Unfortunately, there are quite a few inherent problems with the stress-life approach which cause a large amount of scatter in the experimental fatigue life results. In some companies, due to the extensive use of the stress-life method in past years, a large quantity of S-N curves and experience have been accumulated. In this case, the stress-life method offers compatibility with previous work and may therefore be more appropriate.

• The stress-life approach is still used today for situations which are not easily modeled using the local strain methods, such as welded structures and cast irons. Due to the inherent defects in these materials which act more like cracks, fatigue damage should really be modeled with LEFM crack propagation tools.

Another group of materials which appear to be best modeled using the stress-life approach are

anisotropic and inhomogeneous materials such as composites. However, there are complications even with composites, since the mean stress correction models used in connection with metals do not apply to all composites.

## 9.2.3 Stress Versus Life (S-N) Curves

### Fitting test data for unnotched axial specimens tested under completely reversed loading

## 9.2.3 (S-N) Curves - Forms of Fatigue

• High Cycle Fatigue [HCF]

– Low Amplitude High Frequency Elastic Strain – Tuning Fork Vibration

• Low Cycle Fatigue [LCF]

– High Amplitude Low Frequency Plastic Strain

– Bend Tuning Fork